JOURNAL DE PHYSIQUE IV
Colloque C7, supplCment au Journal de Physique 111, Volume 3, novembre 1993
Materials selection in mechanical design
M.F. ASHBY and D. CEBON
Engineering Design Centre, Engineering Department, TmmpingtonStreet, Cambridge CB2 IPZ, England
A novel materials-selection procedure has been developed and implemented in software. The
procedure makes use of Materials Selection Charts: a new way of displaying material property data;
and performance indices: combinations of material properties which govern performance.
Optimisation methods are employed for simultaneous selection of both material and shape.
The performance of an engineering component is limited by the properties of the material of
which it is made, and by the shapes to which this material can be formed. Under some
circumstances a material can be selected satisfactorily by specifying ranges for individual
properties. More often, however, performance depends on a combination of properties, and then
the best material is selected by maximising one or more 'performance indices'. An example is the
specific stiffness E/p (E is Youngs modulus and p is the density). Performance indices are
governed by the design objectives. One is derived later in this paper and many others are tabulated
elsewhere [ I , 21. Component shape is also an important consideration. Hollow tubular beams are
lighter than solid ones for the same bending stiffness and I-section beams may be better still.
Information about section shape can be included in the performance index to enable simultaneous
selection of material and shape.
A performance index is a group of material properties which governs some aspect of the
performance of a component [I, 21. They are derived from simple models of the function of the
component, as illustrated by the following example.
A material is required for a light, stiff beam. The aim is to achieve a specified bending stiffness at
minimum weight. The beam has a length L and a square, solid, cross-section as shown in Figure
la. The mass of the beam is
where A is the area of the cross-section and p is the density of the material of which the beam is
made. The stiffness S of a simply-su ported beam with modulus E, second moment of area I,
central load F, and central deflection [
Article published online by EDP Sciences and available at http://dx.doi.org/10.1051/jp4:1993701
2 JOURNAL DE PHYSIQUE IV
with C1 = 48 for 3-point bending. Other supports, or other distributions of load, change C1, but
nothing else. Assume that the beam has a square section, of side b. The second moment of area
I = b4/12 = ~ ~ 1 1 2 (3)
The stiffness S and the length L are constrained by the design. The area A is a 'free'
variable that we wish to choose so as to minimise the mass, while meeting the constraints.
F Area A F Y
Fig. 1 (a) A square-section beam loaded in bending
(b) A beam of more complex cross section.
Substituting for I in equation (2) and eliminating A between this and (1) gives
The mass of the beam can be minimised (and perforhance maximised) by seeking the material with
the largest value of the performance index
The same performance index holds for square-section beams with any value of the design stiffness
S, any boundary conditions and distributions of load (defined by Cl), and any length L.
The cross-section shape of the beam (like the I-section shown in Figure lb) can be
included in the performance index by i n d u c i n g a dimensionless shape factor $, defined  by
The value of $ measures the bending efficiency of the section shape. For the solid section of
Figure l(a), $ = 1; that for the I-section of Figure l(b) is about 5. Real I-sections have
efficiencies, $ ,as high as 40. The maximum value of I$ is limited by manufacturing constraints
or by local buckling of the component, and, for this reason, it can be considered to be a material
propeny. Shape factors can also be defined for design against yield or fracture, and for shafts as
well as beams. Using equation (6) in place of equation (3) to eliminate A in equation (1) gives
the new index:
For a constant shape ( $ constant) the criterion reduces to the earlier one; the best selection is then
the material with the largest value of MI (equation (5)). In comparing materials with different
shapes, the best choice is that with the greatest value of M2 (equation (7)).
Material Property Charts
Material selection using performance indices is best achieved by plotting one material
property (or mathematical combination of properties) on each axis of a materials selection chart
[1,2]. In the example shown in Figure 2, the axes are Young's modulus and density. The
logarithmic scales span a range so wide that all materials are included. When data for a given
material class such as metals are plotted on these axes, it is found that they occupy a field which
can be enclosed in a 'balloon'. Ceramics also occupy a field, and so do polymers, elastomers,
composites, and so on. The fields may overlap, but are nonetheless distinct. Individual materials
or sub-classes (like steels, or polypropylenes, PP) appear as little 'bubbles' which define the
ranges of their properties. Hardcopy charts relating many mechanical and thermal properties are
now available [ l ] (two appear in this article). Others can be constructed with the software
described in a moment.
The subset of materials with the greatest value of Mi can be identified rapidly by taking
logarithms of equation (5) (Log E = 2 Log p + 2 Log Mi), and plotting the resulting selection line
of slope 2 on the chart. The construction is illustrated in Figure 2, from which it can be seen that
woods, fibre reinforced composites and some ceramics are the best choices for a light stiff beam
with square crosssection. When section shape is included in the selection criterion, (as in
equation (7)) woods become considerably less attractive, because they cannot be manufactured in
thin sections with large shape factors, like metals. SELECTION LINE
DENSITY, P (Mg/m3)
Fig.2 A modulusldensity chart illustrating the selection of materials with high values of
M I = ~ 1 1 2 1 ~Contours of constant ~ 1 1 2 1appear as a family of lines of slope 2.
Materials with Mi greater than a specified value can be identified
4 JOURNAL D E PHYSIQUE IV
IMPLEMENTATION IN SOFTWARE
The 'Cambridge Materials Selector' (CMS) is a computer package consisting of a data base
of material properties, a management system which recovers and manipulates the data, and a
graphical user interface which presents the property data as material selection charts. The approach
employs a number of novel features [ ]4.
The Selection Process
To select a material, the user performs a series of selection stages. On each stage, a pair of
material properties (or user-definedfunctionsof material properties, like ~ l / ~ / is specified. The
program generates a graph with these properties as the axes. All materials contained in the
database with applicable data entries are plotted on the graph. The area of the graph which satisfies
the selection criterion is specified by the user, and the materials which lie in that area are considered
to have 'passed' the selection stage. Up to six independent selection stages can be performed.
The program stores the results of each selection stage and these can be examined at any
time. It is possible to modify any selection stage so that performance criteria can be tightened or
relaxed until suitable materials are found. A summary of the CMS session can be stored in a disk
file and read into the package later. This enables users to continuelmodify a selection where they
left-off and to re-evaluate the selection criteria in the light of other design information. It also
documents the selection process.
A number of data manipulation routines are available during each selection stage. These
include zooming-in on an area of the graph, listing the properties of particular materials and
displaying the materials which passed all the previous stages. Facilities are available for plotting
hard copies of graphs and listing text information.
Materials, Properties and Data
Three different types of data are stored in the database: (i) Numerical data, (eg density);
(ii) Discrete data (eg material identifier); and (iii) Text data (eg 'typical uses'). Both the
numerical and discrete data types can be plotted, giving three types of materials selection charts:
(i) Charts with two numerical axes like the hand drawn chart of figure 2; (ii) Charts with one
numerical and one discrete axis are 'bar charts'; and (iii) Charts with two discrete properties are
'tables' with each material fitting into one or more cells in the table. The primary, 'generic' CMS
database contains Metals, Polymers, Ceramics, Composites and Natural materials. It contains a
wide range of mechanical, thermal and electrical properties, as well as information on
environmental performance, processing, available forms, typical uses, suppliers, and sources of
further information. The package employs an automatic data checking procedure, which also
ensures that the database is complete [ ] Future versions of the program will handle additional
detailed databases of materials: in particular classes, and for specialised industrial sectors. Several
of these databases are in an advanced stage of development at the time of writing.
Materials for Oars
Boats, before steam power, could be propelled by poling, by sail and by oar. Oars gave
more control than the other two, the military potential of which was well understood by the
Romans, the Vikings and the Venetians. But credit for inventing the rowed boat must no to the
Egyptians: boats with oars appear in carved relief on monumer& built in Egypt between 3300
and 3000 BC.
Mechanically speaking, an oar is a beam loaded in bending. It must be strong enough to
carry the bending moment exerted by the oarsman without breaking, it must have just the right
stiffness to match the rower's own characteristics and give the right "feel", and - very important -
it must be as light as possible. Meeting the strength constraint is easy. Oars are designed on
stiffness, that is, to give a specified elastic deflection under a given load. The upper part of
I LOOM ---------A
Fig. 3 An oar, showing the components and the method of measuring the stiffness.
Figure 3 shows an oar: a blade or "spoon" is bonded to a shaft or "loom" which cames a sleeve
and collar to give positive location in the rowlock. The lower part of the figure shows how the
oar stiffness is measured: a 10 kg weight is hung on the oar 2.05 m from the collar and the
deflection at this point is measured. A soft oar will deflect nearly 50 mm; a hard one only 30. A
rower, when ordering an oar, specifies how hard it should be .
The oar must also be fight; extra weight increases the wetted area of the hull and the drag
that goes with it. So there we have it: an oar is a beam of specified stiffness and minimum
weight. The performance index we want was derived in earlier; it is
What materials make good oars? Figure 2 shows the appropriate chart, with a selection
line for the index placed on it. It identifies three classes of material: woods, carbon- and glass-
fibre reinforced polymers and certain ceramics (Table 1). Ceramics are brittle; they have low
values of toughness; if you dropped a ceramic oar, it would probably shatter. This can be
analysed, leading to further performance indices [l], but there is insufficient space to do so here.
We simply note that ceramics are eliminated because they are brittle and expensive. The
recommendation is clear. Make your oars out of wood or - better - out of CFRP.
TABLE 1 MATERIALS FOR OARS
MATE- M ( ~ ~ a ) ' " / ( ~ g / m ~ )COMMENT
Woods 5-8 Cheap, traditional, but not easily controlled.
CFRP 4-8 As good as wood, more control of properties.
GFRP 3.5-5.5 Cheaper than CFRP but lower M.
Ceramics 4-8 Good M but brittle and expensive
6 JOURNAL DE PHYSIQUE IV
Of what, in reality, are oars made? Racing oars and sculls are made either of wood or of a
high performance composite: carbon-fibre reinforced epoxy, CFRP. Wooden oars are made
today, as they were 100 years ago, by handcraftsmen who use Sitka spruce from the northern US
or Canada, the further north the better because the short growing season gives a finer grain. A
spruce oar weighs between 4 and 4 3 kg, and costs (in 1993)about £150 or $250. Composite
blades are a little lighter than wood, for the same stiffness. The component parts are fabricated
from a mixture of carbon and glass fibres in an epoxy matrix, assembled and glued. The
advantage of composites lies partly in the saving of weight (typical weight: 3 9 kg) and partly in
the greater control of performance: the shaft is moulded to give the stiffness specified by the
purchaser. At a price, of course: a CFRP oar costs about £300 ( 4 0 .
Materials for Precision Instruments
The precision of a measuring device, like a sub-micrometerdisplacement gauge, is limited
by its stiffness, and by the dimensional change caused by temperature gradients. Compensation
for elastic deflection can be arranged, and corrections to cope with thermal expansion are possible
too - provided the device is at a uniform temperature. Thermal gradients are the real problem: they
cause a change of shape - that is, distortion - of the device for which compensation is not possible.
Sensitivity to vibration is also a problem: natural excitation introduces noise into the measurement.
So - in precision instrument design - it is permissible to allow expansion, provided distortion does
not occur [61. Elastic deflection is allowed, provided natural vibration frequencies are high.
What, then, are good materials for precision devices?
Figure 4 A precision instrument. It consists of a force loop, an actuator and a sensor
Figure 4 shows, schematically, such a device: it consists of a force loop, an actuator and a
sensor; we aim to choose a material for the force loop. It will, in general, support heat sources:
electrical components which generate heat. The relevant performance index is found by
considering the simple case of one-dimensional heat flow through a rod insulated except at its
ends, one of which is at ambient and the other connected to the heat source. In the steady state,
Fourier's law is
where q is heat input per unit area, h is the thermal conductivity and -
is the resulting
temperature gradient. The strain is related to temperature by
where a is the thermal conductivity and To is ambient temperature, from which
Thus for a given geometry and heat flow, the distortion dE/& is minimised by selecting materials
with large values of the index
0.01 0.1 1 10 100 1000
THERMAL CONDUCTIVITY A w / ~ K )
Figure 5. A Chart of thermal conductivity, h, and expansion coefficient, a, allowing selection of
materials for the force loop of precision instruments.
8 JOURNAL D E PHYSIQUE IV
The other problem is vibration. The sensitivity to external excitation is minimised by making the
natural frequencies of the device as high as possible. The flexural vibrations have the lowest
frequencies; they are proportional, once again, to
A high value of this index will minimise the problem. Finally, of course, the device must not cost
Chart 10 (Figure 5) shows the expansion coefficient, a,plotted against the thermal
conductivity, 1 Contours show constant values of the quantity hla. A search region is isolated
by the line Wa = lo7 W/m, giving the short list of Table 2. Values of MI = Eln/p read from
Chart 1 (Figure 2) are included in the table.
TABLE 2 MATERIALS TO MINIMISE T'HERMAL DISTORTION
MATERIAL M3 =hla M, = E~~~ COMMENT
DIAMOND 5 x lo8 8.6 Outstanding MI and M3;
SILICON 4 lo7 6.0 Excellent M1 and &;cheap.
SILICON CARBIDE 2.107 6.2 Excellent MI and M3; potentially
BERYLLIUM lo7 9 Less good than silicon or Sic.
ALUMINIUM lo7 3.1 Poor MI, but very cheap.
SILVER 2 x lo7 1.O ) High density
COPPER 2 lo7 1.3 gives poor
GOLD 2 x lo7 0.6 ) value of MI.
TUNGSTEN 3 x lo7 1.1 ) Better than copper, silver or
MOLYBDENUM 2 x lo7 1.3 ) gold, but less good than
WAR 3 x lo7 1.4 ) silicon, Sic, diamond
Diamond is outstanding, but practical only for very small devices. The metals, except for
beryllium, are disadvantaged by having high densities and thus poor values of MI = E. '% The
best choice is silicon, available in large sections, with high purity. Silicon carbide is an alternative.
Nano-scale measuring and imaging systems present the problem analysed here. The
atomic-force microscope and the scanning-tunnelling microscope both support a probe on a force
loop, typically with a piezo-electric actuator and electronics to sense the proximity of the probe to
the test surface. Closer to home, the mechanism of a video recorder and that of a hard disk drive
qualify as precision instruments; both have an actuator moving a sensor (the read head) attached,
with associated electronics, to a force loop. The materials identified in this case study are the best
choice for force loop.
A novel materials selection procedure has been implemented in software. It contains a database of
quantitative and qualitative data for a wide range of engineering materials: metals, polymers,
ceramics, composites and natural materials. The management system provides an interactive
graphical selection environment suitable for mechanical engineering design, employing
performance indices for selecting materials with optimum properties and section shape.
The authors are very grateful to the Leverhulme Trust for funding development of the Cambridge
Materials Selector, and to Ruth Thomas for her assistance with development of the user interface.
[I] Ashby, MF. 'Materials selection in mechanical desin' Pergamon Press, Oxford, 1992.
[21 Ashby, MF. 'On the engineering properties of materials' Acta Metal-, 37, p1273, 1989.
131 Ashby, MF. 'Materials and shape' Acta Metallurb, 39, 1025 , 1991.
 Cebon, D and Ashby, MF. 'Computer-based materials selection for mechanical design' in
'Computerization and networking of materials databases', ASTM STP 1140, American
Society for Testing and Materials, Philadelphia, 1992.
 Redgrave, S "Complete Book of Rowing", Partridge Press, London (1992).
[61 Chetwynd, D.G. (1987) Precision Engineering, 2, (I), 3.